Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- Indent Tests for Explosive Equation... by Altair Engineering 1073 views
- Verification of johnson cook materi... by eSAT Publishing H... 595 views
- Finite Element Simulation of Serrat... by IJRES Journal 507 views
- BAV Budapest, Márkareggeli - Trust by BAVBudapest 451 views
- BAV - Az Új Trónkövetelők by Laszlo Aczel 336 views
- Izgalmas személyiség, differenciált... by Zoltán Vasvári 845 views

No Downloads

Total views

717

On SlideShare

0

From Embeds

0

Number of Embeds

1

Shares

0

Downloads

16

Comments

0

Likes

1

No embeds

No notes for slide

- 1. International Journal of Plasticity 26 (2010) 1746–1771 Contents lists available at ScienceDirect International Journal of Plasticity journal homepage: www.elsevier.com/locate/ijplasA plastic constitutive equation incorporating strain, strain-rate,and temperatureJi Hyun Sung a, Ji Hoon Kim b, R.H. Wagoner c,*a Department of Mechanical Engineering, The Ohio State University, 2041 College Road, Columbus, OH 43210, USAb Materials Deformation Group, Korea Institute of Materials Science, 531 Changwondaero, Changwon, Gyeongnam 641-831, South Koreac Department of Materials Science and Engineering, The Ohio State University, 2041 College Road, Columbus, OH 43210, USAa r t i c l e i n f o a b s t r a c tArticle history: An empirical plasticity constitutive form describing the ﬂow stress as a function of strain,Received 24 November 2009 strain-rate, and temperature has been developed, ﬁt to data for three dual-phase (DP)Received in ﬁnal revised form 12 February 2010 steels, and compared with independent experiments outside of the ﬁt domain. DubbedAvailable online 15 March 2010 the ‘‘H/V model” (for ‘‘Hollomon/Voce”), the function consists of three multiplicative func- tions describing (a) strain hardening, (b) strain-rate sensitivity, and (c) temperature sensi-Keywords: tivity. Neither the multiplicative structure nor the choice of functions (b) or (c) is novel. TheConstitutive equation strain hardening function, (a), has two novel features: (1) it incorporates a linear combina-Work hardeningDual-phase (DP) steel tion coefﬁcient, a, that allows representation of Hollomon (power law) behavior (a = 1),Thermal–mechanical FE simulation Voce (saturation) behavior (a = 0) or any intermediate case (0 < a < 1, and (2) it allowsDeformation-induced heating incorporation of the temperature sensitivity of strain hardening rate in a natural way by allowing a to vary with temperature (in the simplest case, linearly). This form therefore allows a natural transition from unbounded strain hardening at low temperatures toward saturation behavior at higher temperatures, consistent with many observations. Hollomon, Voce, H/V models and others selected as representative from the literature were ﬁt for DP590, DP780, and DP980 steels by least-squares using a series of tensile tests up to the uniform strain conducted over a range of temperatures. Jump-rate tests were used to probe strain rate sensitivity. The selected laws were then used with coupled thermo-mechanical ﬁnite element (FE) modeling to predict behavior for tests outside the ﬁt range: non-isother- mal tensile tests beyond the uniform strain at room temperatures, isothermal tensile tests beyond the uniform strain at several temperatures and hydraulic bulge tests at room tem- perature. The agreement was best for the H/V model, which captured strain hardening at high strain accurately as well as the variation of strain hardening with temperature. The agreement of FE predictions up to the tensile failure strain illustrates the critical role of deformation-induced heating in high-strength/high ductility alloys, the importance of hav- ing a constitutive model that is accurate at large strains, and the implication that damage and void growth are unlikely to be determinant factors in the tensile failure of these alloys. The new constitutive model may have application for a wide range of alloys beyond DP steels, and it may be extended to larger strain rate and temperature ranges using alternate forms of strain rate sensitivity and thermal softening appearing in the literature. Ó 2010 Elsevier Ltd. All rights reserved. * Corresponding author. Tel.: +1 614 292 2079; fax: +1 614 292 6530. E-mail address: wagoner.2@osu.edu (R.H. Wagoner).0749-6419/$ - see front matter Ó 2010 Elsevier Ltd. All rights reserved.doi:10.1016/j.ijplas.2010.02.005
- 2. J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 17471. Introduction Advanced high strength steels (AHSS) provide remarkable combinations of strength and ductility by careful control ofmicrostructure of ferrite, martensite, and retained austenite components. Dual-phase (DP) steel microstructures consist oflarge islands (of approximately the grain size) of hard martensite embedded in a softer ferrite matrix, thus mimicking a typ-ical discontinuous composite structure. DP steels are well-established but their widespread adoption has been limited be-cause die tryouts show that forming failures can occur much earlier than predicted using standard forming limitdiagrams (FLD) and commercial ﬁnite element (FE) programs. Unlike failures observed with traditional steels, unexpectedDP steel failures occur in long channel regions of low R/t (bending radius/sheet thickness) as the sheet is drawn over thedie radius while being stretched, bent and straightened. Such failures are often dubbed ‘‘shear fracture” by industrial prac-titioners (Huang et al., 2008; Sklad, 2008; Chen et al., 2009). Conventional wisdom has attributed this phenomenon to a spe-cial damage/void growth mechanism, possibly related to the large, hard martensite islands (Takuda et al., 1999; Horstemeyeret al., 2000; Lee et al., 2004; Sarwar et al., 2006; Wagoner, 2006; Vernerey et al., 2007; McVeigh and Liu, 2008; Xue, 2008;Sun et al., 2009). Recent work was conducted by the authors to determine whether such unpredicted forming failures are a result of typicalplastic localization or a special kind of fracture. Draw-bend tests which reproduce the conditions that promote ‘‘shear fail-ure” were found to exhibit greatly varying formability depending on the strain rate in the test (Wagoner et al., 2009a,b). Fur-thermore, temperatures of up to 100 °C in sheet regions away from the necking area were measured, much higher than withtypical traditional steels with lower strength/ductility combinations. It became apparent that the role of temperature in theﬂow stress, almost universally ignored in standard sheet forming simulations and mechanical property determinations,might be a critical factor. In order to consider these effects quantitatively, a reliable constitutive equation was needed inthe range of strain, strain rate, and temperature encountered in such tests and forming operations.1.1. Role of deformation-induced heating in plastic localization Unlike the uniformly elevated temperature imposed in a warm forming process (usually applied to increase the inherentductility of the alloy), the heat caused by plastic deformation in a local region of high strain has a detrimental effect onmechanical formability because most alloys soften with increasing temperature, and the softening occurs at the eventualfracture location (Kleemola and Ranta-Eskola, 1979; Ayres, 1985; Lin and Wagoner, 1986; Gao and Wagoner, 1987; Linand Wagoner, 1987; Wagoner et al., 1990; Ohwue et al., 1992). The phenomenon can be seen as a kind of ‘‘reversestrain-rate sensitivity,” because the higher strain rate in an incipient or developed neck tends to increase the ﬂow stressvia strain-rate sensitivity (and thus delay failure) but also tends to decrease the ﬂow stress via the material’s temperaturesensitivity (thus promoting earlier failure) (Wagoner and Chenot, 1997; Ghosh, 2006). The deformation-induced thermal effects are important at strain rates high enough that heat transfer out of the neck re-gion is limited. At sufﬁciently low rates the deformation becomes quasi-isothermal and temperature sensitivity has a neg-ligible effect. At sufﬁciently high rates the deformation is quasi-adiabatic and the heat stays where it is generated. Typicalsheet-forming strain rates in the automotive industry are approximately 10/s (Fekete, 2009), which is close to the adiabaticlimit for typical steels. Therefore, the role of temperature sensitivity of ﬂow stress may be important if it is sufﬁciently highand the work of deformation (related to ﬂow stress times ductility) is sufﬁcient to raise the temperature signiﬁcantly. For DPsteels with high strength and ductility, an accurate description of ﬂow stress incorporating temperature may be essential.Such a description, if veriﬁed, may also be useful for a large range of other materials and applications.1.2. Plastic constitutive equations The number, range and complexity of plastic constitutive equations proposed for metals are formidable. They take manyforms, depending on application and intent. The application of interest in the current work is metal forming, sheet metalforming to be more precise. Typical sheet metal formability is related to the resistance to tensile necking, which is in turnrelated to the evolution of plastic ﬂow stress in biaxial tensile stress states encountered during the progressive forming.Through-thickness stress is typically close to zero (i.e. plane stress) until failure is imminent. Multi-axial aspects of the plastic constitutive response (yield surface shape, size, and location evolution) are often sepa-rated for convenience from one-dimensional (1-D) aspects that are obtainable from tensile tests carried out at various strainrates and temperatures. The current interest is in 1-D aspects. Since many material elements undergo strain paths close toproportional, strain reversal effects such as the Bauschinger effect can be ignored for many applications. The preponderance of sheet metal forming is carried out at moderate strain rates (up to approximately 10/s (Fekete,2009)) and nominally room temperature (although excursions of the order of up to 100 °C are possible because of heat gen-erated deformation and friction during forming (Wagoner et al., 2009a,b)). For most sheet-formed metals of commercialinterest (e.g. steel, aluminum, copper, titanium) under these conditions, strain hardening is the primary material factorresisting necking, with strain-rate and temperature sensitivity of ﬂow stress being secondary. As listed in Appendix A, there are integrated constitutive equations relating plastic ﬂow stress with strain, strain rate, andtemperature (which is the focus of the current work). The strain hardening representations (at constant strain rate and
- 3. 1748 J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771temperature) are of two main types (Table 1): those that approach a saturation stress at large strain (e.g. Brown–Anand(‘‘BA”) model (Anand, 1982, 1985; Brown et al., 1989), MTS model (Kocks, 1976; Mecking and Kocks, 1981; Follansbeeand Kocks, 1988), Modiﬁed Bodner–Partom (‘‘BP”) model (Bodner and Partom, 1975; Chen et al., 2008) and Lin-Wagoner(‘‘LW”) Model (Lin and Wagoner, 1987)) and those that are unbounded at large strain (e.g. Zirilli–Armstrong (‘‘ZA”) model(Zerilli and Ronald, 1987), Rusinek–Klepaczko (‘‘RK”) model (Klepaczko, 1987; Rusinek and Klepaczko, 2001; Rusineket al., 2007) and Khan–Huang–Liang (‘‘KHL”) model (Khan and Huang, 1992; Khan and Liang, 1999; Khan and Zhang,2000, 2001; Khan et al., 2004; Khan et al., 2007)). The ﬁrst group may be called, in short, ‘‘saturation” or ‘‘Voce” models (Voce,1948; Follansbee and Kocks, 1988) while the second may be called ‘‘Hollomon” or ‘‘power-law” models (Hollomon, 1945);the proper names refer to the simplest empirical versions of these strain hardening forms appearing in the literature, withthree parameters or two parameters, respectively. The saturation-type laws are typically found suitable for materials at higher homologous temperatures (and most face-centered cubic (FCC) metals such as aluminum and copper (Mishra et al., 1989; Choudhary et al., 2001) at room temperature)while power-law-type models are more suitable for body-centered cubic (BCC) metals and at low homologous temperatures.For example, iron alloys are known to continue strain hardening at strains up to at least 3 (Johnson and Holmquist, 1988). Integrated constitutive equations may be subdivided in another way: those that accommodate strain hardening ratechanges with temperature changes (e.g. BA model, MTS model, Modiﬁed BP model, LW Model and RK model) and those thatdo not (e.g. ZA model and KHL model), Table 1. As shown in Table 1, only the saturation-type integrated laws incorporatestrain hardening rates that are sensitive to temperature (beyond ﬁxed multiplicative or additive functions), with one excep-tion: the RK model. The RK model (2001) incorporates power-law strain hardening with a power, n, that varies in a pre-scribed manner with temperature as shown in Appendix A. It is similar in concept to the LW model (1987), where strainhardening parameters in a saturation-like law are allowed to vary linearly with temperature, thus using six material param-eters (Appendix A). In addition to the integrated constitutive equations mentioned above, there are myriad ways to choose and combineotherwise independent basis functions of strain, strain rate and temperature, which may be generally represented as f(e),gðeÞ, and h(T), respectively, where e is true tensile strain, e is true strain rate, and T is temperature. (See Appendix B for a _ _list of typical functions if this kind. The total number of multiplicative combinations for the choices presented there aloneis 126.) The basis functions may be combined multiplicatively (Hutchison, 1963; Kleemola and Ranta-Eskola, 1979; Johnsonand Cook, 1983; Lin and Wagoner, 1986), additively (Wagoner, 1981b; Ghosh, 2006), or by some combination (Zerilli andRonald, 1987) thereof. Each material model of these types prescribes the strain hardening at each temperature as a simplemultiple or addition (or combination), rather than allowing for the character or rate of strain hardening to vary with tem-perature, hence the deﬁnition adopted for Table 1 to decide whether strain hardening is a function of temperature or not.Common choices for the basis functions f(e), gðeÞ, and h(T), are presented in Appendix B. Several of these combinations have _been reviewed and ﬁt to tensile data in the literature (Lin and Wagoner, 1986).1.3. Purpose of the current work The purpose of the current work is to develop and verify an empirical plastic constitutive model that meets the followingconditions while introducing the minimum number of undetermined parameters: (1) it reproduces strain hardening accurately at large strain from ﬁtting in the uniform tensile range, (2) it captures both extreme kinds of strain hardening forms as well as intermediate cases: bounded (power law) and unbounded (saturation), (3) it captures the change of strain hardening character and rate depending on temperature, and (4) it is capable of predicting strain localization and failure under typical sheet forming conditions of strains, strain rates, and temperatures. In order to accomplish these goals, a new multiplicative type phenomenological constitutive equation, the H/V model, isintroduced. The H/V model is a linear combination of the Hollomon and Voce strain hardening equations with a tempera-Table 1Classiﬁcation of integrated 1-D plastic constitutive equations that incorporate the effects of strain, strain-rate, and temperature.a Unbounded-stress at large strain Strain hardening change with temperature Brown–Anand N Y MTS N Y Modiﬁed Bodner–Partom N Y Lin–Wagoner N Y Zirilli–Armstrong Y N Khan–Huang–Liang Y N Rusinek–Klepaczko Y Y a For the classiﬁcation shown in Table 1, whenever the ﬂow stresses for a given strain at two temperatures differ only by a constant ratio or difference,then the strain hardening rate is deemed not to depend on temperature.
- 4. J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 1749ture-dependent proportion. The temperature-dependent proportion represents the change of strain hardening character andrate as temperature changes. Standard multiplicative forms for strain rate sensitivity and thermal softening are incorporatedfor ﬁtting and testing. The initial application, the one for which testing is conducted, is for sheet metal forming at rates up to10/s with deformation-induced heating to temperatures up to 100 deg. C. These are conditions normally encountered innominally room-temperature pressforming operations; the application that inspired the current work. Nonetheless, theH/V model may have application outside of this regime with or without changes in forms to accommodate larger rangesof strain rate and temperature.2. H/V constitutive equation A new empirical work hardening constitutive model, H/V model, is proposed as three multiplicative functions, Eq. (1). r ¼ rðe; e; TÞ ¼ f ðe; TÞ Á gðeÞ Á hðTÞ _ _ ð1Þ Functions f, g, and h together represent the effects of strain, strain rate, and temperature, respectively, on the tensile ﬂowstress r. g and h are chosen from any of several standard forms (see Appendix B), but the strain hardening function, f, is no-vel: it incorporates the temperature sensitivity of strain hardening rate via a linear combination of Voce (saturation) (1948)and Hollomon (power-law) (1945) strain-hardening forms.2.1. Strain hardening function, f(e,T) The function f(e, T) represents the major departure and contribution of the new development. The motivation for thedevelopment of f(e, T) is illustrated in Fig. 1(a), which shows strain hardening curves for a dual-phase steel, DP 780, at threetemperatures. To compare the strain hardening curve shapes, the stresses are normalized by dividing by the yield stresses ateach temperature, Fig. 1(b). Clearly the strain hardening rate varies with temperature, being lower at higher temperatures.This behavior, which is seldom captured by existing constitutive models, is one of the two principal motivations for the cur-rent development. In this study, a strain hardening function f(e, T) of the following form is proposed: f ðe; TÞ ¼ aðTÞfH þ ð1 À aðTÞÞ Á fV ð2Þ 8 > aðTÞ ¼ a1 À a2 ðT À T 0 Þ < f ¼ HHV enHV ð3Þ > H : fV ¼ V HV ð1 À AHV eÀBHV e Þwhere T0 is a reference temperature (298 K for simplicity), and a1a2, HHV, nHV, VHV, AHV, and BHV are material constants. Thefunction a(T) allows a more Voce-like curve at higher temperatures, and a more Hollomon-like curve at lower temperaturesor vice versa, depending on the sign of a1. If a(T) = 1, the H/V model becomes a pure Hollomon model and if a(T) = 0 it be-comes a pure Voce model. If an intermediate hardening rate is sought that does not depend on temperature, a may be chosento be constant: 0 < a0 < 1.2.2. Strain rate sensitivity function gðeÞ, temperature sensitivity function h(T) _ The functions gðeÞ and h(T) within the H/V model are not novel; the exact form may be selected from among those _appearing in the literature, as listed in Appendix B, or as otherwise devised. It is anticipated that the choice of form of thesefunctions will not be important over the range of strain rates (up to 10À1/s) and temperatures (25–100 °C) encountered in thetesting carried out in the current work. For extended ranges, the choice of gðeÞ and h(T) may become more clear. The choices _of terms gðeÞ and h(T) for the implementation of the H/V model tested in the current work will be explained in more detail in _Section 4.1.3. Experimental procedures The experiments were chosen to correspond to typical sheet forming practice applied to three DP steels representing arange of strengths typical of automotive body applications. Constitutive models were ﬁt using standard tensile tests up tothe uniform strain. The quality of the ﬁts was then probed using tensile tests and hydraulic bulge tests to failure.3.1. Materials DP steels exhibit good formability and high strength derived from a microstructure that is a combination of a soft ferritematrix and a hard martensite phase ‘‘islands.” Three grades of DP steels of nominally 1.4 mm thickness, DP590, DP780, andDP980, were provided by various suppliers, who requested not to be identiﬁed. DP590 was supplied without coating, DP780with hot-dipped galvanized coating (HDGI), and DP980 with hot-dipped galvanneal coating (HDGA). The chemical
- 5. 1750 J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 1000 25 deg.C 750 50 deg.C True Stress (MPa) 100 deg.C 500 250 DP780 -3 dε/dt: 10 /s 0 0 0.05 0.1 0.15 True Strain (a) 2 25 deg.C Normalized True Stress 50 deg.C 100 deg.C 1.5 DP780 -3 dε/dt: 10 /s 1 0 0.05 0.1 0.15 True Strain (b)Fig. 1. Stress–strain response of DP780 at three temperatures: (a) experimental curves and (b) the same data, replotted with the stress divided by the initialyield stress to reveal strain-hardening differences.compositions were determined utilizing a Baird OneSpark Optical Emission Spectrometer (HVS-OES) based on ASTM E415-99a(05) and standard tensile tests were carried out according to ASTM E8-08 at a crosshead speed of 5 mm/min. Both kindsof tests were conducted at General Motors North America (GMNA, 2007). The chemical compositions and standard ASTMstandard tensile properties appear in Tables 2 and 3, respectively. In order to distinguish normal anisotropies measured fromsheets of the original thickness and those thinned for balanced biaxial testing (as will be discussed in Section 3.5), symbols r1and r2 in Table 3 refer to sheets of original thickness and thinned thickness, respectively.Table 2Chemical composition of dual-phase steels in weight percent (balance Fe).a C Mn P S Si Cr Al Ni Mo Nb Ti V B DP590 0.08 0.85 0.009 0.007 0.28 0.01 0.02 0.01 <.01 <.002 <.002 <.002 <.0002 DP780 0.12 2.0 0.020 0.003 0.04 0.25 0.04 <.01 0.17 <.003 <.003 <.003 <.0002 DP980 0.10 2.2 0.008 0.002 0.05 0.24 0.04 0.02 0.35 <.002 <002 <.002 <.0002 a Chemical analysis was conducted at General Motors North America (GMNA, 2007).
- 6. J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 1751Table 3Mechanical properties of dual-phase steels.a Thickness (mm) 0.2% YS (MPa) UTS (MPa) eu (%) et (%) nb Dr c r1c r2 d ad DP590 1.4 352 605 15.9 23.2 0.21 0.30 0.84 0.98 1.83 DP780 1.4 499 815 12.7 17.9 0.19 À0.11 0.97 0.84 1.86 DP980 1.4 551 1022 9.9 13.3 0.15 À0.23 0.76 0.93 1.90 a Tests were conducted at General Motors North America (GMNA, 2007) with 5 mm/min crosshead speed at room temp except for test of r2 and a whichwere conducted at Alcoa (ATC, 2008; Brem, 2008) with thinned materials. b n value was calculated from an engineering strain interval of 4–6%. c Dr and r1 were calculated at the uniform strain of original thickness material using Dr = (r0 À 2r45 + r90)/2 and r = (r0 + 2r45 + r90)/4, respectively. d r2 value was calculated at the uniform strain of thinned materials using r = (r0 + 2r45 + r90)/4 and a was found by the ﬁt of bulge test result to tensile testdata (using Eq. (9)) considering anisotropy (r2) of thinned materials.3.2. Material variation In order to assure uniform, reproducible material properties in this work, a study was undertaken to determine variationsof mechanical properties across the width of a coil. DP steels can exhibit more signiﬁcant variations in this regard (as com-pared with traditional mild or HSLA steels) because of the complex thermo-mechanical treatment they undergo during pro-duction, Fig. 2. The standard deviation of the ultimate tensile stress for DP590 was 25 MPa, a scatter greater than 4% of theaverage UTS. In order to quantify the spatial distribution of material properties and with a goal to minimize such effects on subsequenttesting, numerous rolling direction (RD) tensile tests were conducted with simpliﬁed rectangular (non-shouldered) tensilespecimens of DP590 having gage regions between the grips of 125 mm Â 20 mm. (As will be shown later, see Fig. 4, useof the rectangular specimens introduces no signiﬁcant errors up to the uniform elongation.) In order to minimize the effectof sheared edge quality, the specimen edges were smoothed with 120 grit emery cloth (a practice that was followed for alltensile tests used in this work). The results from these specimens are summarized in Fig. 3: specimens within 360 mm of thecoil edge (and thus more than 390 mm from the coil center line) exhibit systematic and signiﬁcant variations in thicknessand UTS, while those in the central region do not. A similar set of tests was performed for a DP980 steel (not the one usedelsewhere in the current work) with the coil width of 1500 mm. The central region more than 300 mm from the edges haduniform properties. For the three materials used in the current work, DP590 (coil width 1500 mm), DP780 (coil width1360 mm), DP980 (coil width 1220 mm), only material at least 360 mm from the coil edges was used.3.3. Tensile testing ASTM E8-08 sheet tensile specimens with 0% and 1% width taper were initially used for tensile testing, but failures oc-curred frequently outside of the gage region, thus making the consistent measurement of total elongation problematic.The failures outside of the gage region were more prevalent at elevated temperatures. In order to obtain consistent test re-sults, the width taper was increased to 2%, which proved sufﬁcient to insure failure at the center of the specimen for all tests.As expected (Raghavan and Wagoner, 1987), the increased taper reduced the total elongation, but there was no signiﬁcanteffect on stress–strain measurement up to the uniform elongation, Fig. 4. The consistency and reproducibility of tensile results after these two improvements, that is, using material from the cen-ter of the coil and specimens with 2% width tapers, are illustrated in Fig. 5. The standard variation of UTS is less than 2 MPa 800 Engineering Stress (MPa) 600 σ =567MPa UTS 400 S.D.=25MPa 200 DP590 Strain rate: 10-2 /s 0 0 5 10 15 20 25 30 Engineering Strain (%) Fig. 2. Typical range of tensile behavior for DP590 steel specimens selected from various positions across the width of a coil.
- 7. 1752 J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 1.5 DP590 σ =621MPa 640 UTS 1.47 dε/dt: 10 /s -3 S.D.=2MPa (0.3%) Thickness (mm) 620 UTS (MPa) 1.44 UTS 600 360mm 1.41 580 1.38 Thickness 560 1.35 0 100 200 300 400 500 600 700 Distance from coil edge (mm) Fig. 3. Variation of sheet thickness and ultimate tensile strength with position from the edge of a coil (coil width of 1500 mm). 800 Rectangular Specimen Engineering Stress (MPa) 600 2% Taper Shouldered 1% Taper Specimen 400 No Taper 200 DP590 -3 dε /dt: 10 /s 0 0 0.1 0.2 0.3 Engineering Strain Fig. 4. Effect of tensile specimen geometry on measured stress–strain curves. 1000 DP980 σ = 972MPa, S.D.= 2MPa Engineering Stress (MPa) UTS e =0.139, S.D.= 0.002 f 800 DP780 σ =796MPa, S.D.= 2MPa UTS e =0.176, S.D.= 0.002 f 600 DP590 σ = 624MPa, S.D.= 0.7MPa UTS e =0.247, S.D.= 0.006 f 400 4 tests per material 2% tapered specimen -3 dε/dt: 10 /s 200 0 0.1 0.2 0.3 Engineering StrainFig. 5. Consistency and scatter of tensile results for three DP steels using 2% tapered tensile specimens and material at least 360 mm away from the edge ofthe coil.(less than 0.3 % of the average value for each material), and the variation of the total elongation is less than 0.006 (less than2.5% of the average value for each material). In view of these results, specimens with 2% tapers cut from the central region ofthe coil were used for all subsequent tensile testing.
- 8. J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 1753 For ﬁnding the parameters for the selected constitutive equations, isothermal tensile tests were conducted at 25 °C, 50 °C ,and 100 °C using a special test ﬁxture designed for tension–compression testing (Boger et al., 2005; Piao et al., 2009). In thisapplication, the side plates that are pressed against the surface of the specimen (with a force of 2.24 kN) were not required tostabilize the specimen mechanically against buckling but served instead to heat the specimen for the 50 °C and 100 °C testsand to maintain near-isothermal conditions throughout the contact length and testing time for all tests. For strain rates up to10À3/s, the temperature measured in the gage length of the specimen using embedded thermocouples was maintained with-in 1 °C of the original one up to the uniform strain for all three materials. This method has several advantages compared withperforming tensile tests in air in a furnace, including rapid heat-up (about 3 min to achieve 250 °C), uniform temperaturealong the length, and direct strain measurement using a laser extensometer. The data was corrected for side plate friction (which was minimized using Teﬂon sheets) and the slight biaxial stress (whichwas about 1.5 MPa) using procedures presented elsewhere (Boger et al., 2005). The friction coefﬁcient was determined from theslope of a least-squares line through the measured maximum force vs. four applied side forces (0, 1.12, 2.24 and 3.36 kN). Thefriction coefﬁcients obtained in this way were 0.06, 0.05 and 0.06 for DP590, DP780 and DP980, respectively. Examples of the tensile testing data at a strain of 10À3/s illustrate the effect of test temperature on the stress–straincurves (Fig. 6), the yield and ultimate tensile stresses (Fig. 7), and the uniform and total elongations (Fig. 8). The reducedelongation to failure of higher temperatures is a direct consequence of the lower strain hardening. For the purpose of comparison with FE simulation, non-isothermal tensile tests were also conducted at a strain rate of10À3/s in air at room temperature.3.4. Strain rate jump tests For materials with limited strain rate sensitivity relative to strength, even small differences of strength from specimen-to-specimen introduce large relative errors. Jump-rate tensile tests remove specimen-to-specimen variations and thus are pre-ferred under these conditions. Strain rate jump-down tests, i.e. abruptly changing from a higher strain rate to lower strainrate, were employed in this study. (Stress–relaxation tests can also remove specimen variations but usually can only be usedfor very low strain rates, less than 10À6/s (Wagoner, 1981b).) Fourteen down-jump rate changes, with one jump per tensiletest (Saxena and Chatﬁeld, 1976), were conducted at engineering strains of 0.1, 0.08, 0.06 for DP590, DP780, and DP980steels, respectively, using the following pairs of rates: 0.5/s ? 0.1/s, 0.5/s ? 0.05/s, 0.1/s ? 0.01/s, 0.1/s ? 0.001/s, 0.05/s ? 0.01/s, 0.05/s ? 0.005/s, 0.01/s ? 0.001/s, 0.001/s ? 0.0001/s. The jumps 0.1/s ? 0.01/s, 0.01/s ? 0.001/s and 0.001/s ? 0.0001/s were repeated three times. It has been shown that strain rate sensitivity is nearly independent of strain forsteels (Wagoner, 1981a), which makes jump tests at a single intermediate strain sufﬁcient. For each down jump, a logarithmic strain rate sensitivity value was determined from the ﬂow stresses r1 and r2 at thetwo strain rates e1 and e2 , respectively, for an average strain rate of the two tested strain rates as shown: _ _ r2 e2 m _ lnðr2 =r1 Þ ¼ !m¼ ð4Þ r1 e1 _ lnðe2 =e1 Þ _ _ pﬃﬃﬃﬃﬃﬃﬃﬃﬃ e _ av erage ¼ e1 e2 _ _ ð5Þ The stress after the jump shows a transient response that can be minimized by extrapolating both the higher rate curveand the lower rate curve to a common true strain 0.005 beyond the jump strain, at which point r1 and r2 are found (Wag-oner, 1981a). The procedure is illustrated in Fig. 9 for the case of DP590 with a jump from 10À1/s to 10À2/s. The response atthe higher ﬁrst strain rate over a true strain range of 0.02 is ﬁt to a fourth-order polynomial and extrapolated to the common 800 Engineering Stress (MPa) Room Temp. 600 o o o 100 C 75 C 50 C 400 200 DP590 -3 dε/dt: 10 /s 0 0 0.1 0.2 0.3 Engineering Strain Fig. 6. Variation of strain hardening and failure elongation of DP590 with test temperature.
- 9. 1754 J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 50 50 DP780 -3 dε /dt: 10 /s σ σ (MPa) (MPa) 0 y 0.13 0 y σ UTS 0.27 0.34 25 deg.C 25 deg.C σ UTS σ- σ σ- σ -50 -50 0.90 DP590 -3 dε /dt: 10 /s -100 -100 25 50 75 100 25 50 75 100 T (deg. C) T (deg. C) (a) (b) 50 DP980 dε /dt: 10-3 /s (MPa) 0 σ y 25 deg.C σ 0.48 UTS σ- σ -50 0.76 -100 25 50 75 100 T (deg. C) (c) Fig. 7. Variation of yield stress and ultimate tensile stress with test temperature: (a) DP590, (b) DP780 and (c) DP980.strain. The response at the second lower strain rate is similarly ﬁt to a strain range of 0.02 starting at a true strain 0.01 higherthan the jump strain, and is extrapolated to the common strain. The stresses from these extrapolated curves at the commonstrain are used to determine the m value from Eq. (4).3.5. Hydraulic bulge tests Hydraulic bulge tests were conducted at the Alcoa (ATC, 2008). Because of force limits of the ATC hydraulic bulge testsystem, the materials were machined from one side, from an as-received thickness of 1.4 mm–0.5 mm. The stress–strainresponse of thinned materials was within standard deviations of 5–10 MPa of the original thickness materials dependingon the material. The die opening diameter was 150 mm and the die proﬁle radius was 25.4 mm. For materials that exhibitin-plane anisotropy, the stress state near the pole is balanced biaxial tension (Kular and Hillier, 1972) with through-thick-ness stress negligible for small thickness/bulge diameter ratios (Ranta-Eskola, 1979). In-plane membrane stress, rb, and themagnitude of thickness strain, et, are given by Eq. (6) and Eq. (7), respectively. pR rb ¼ ð6Þ 2t D et ¼ 2 ln ð7Þ D0where p is pressure, R is a radius of bulge, t is current thickness, D is current length of extensometer, and D0 is the initiallength of the extensometer, 25.4 mm. The radius of curvature R, is measured using a spherometer with each leg locatedat a ﬁxed distance of 21.6 mm from the pole. More detailed information for the Alcoa testing machine has appeared else-where (Young et al., 1981).
- 10. J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 1755 0.2 -3 dε/dt: 10 /s Temp: 25 deg. C Uniform Elongation, e u DP590 0.15 DP780 DP980 0.1 25 50 75 100 T (deg. C) (a) 0.3 -3 dε/dt: 10 /s Temp: 25 deg. C f Total Elongation, e DP590 0.2 DP780 DP980 0.1 25 50 75 100 T (deg. C) (b) Fig. 8. Ductility change with temperature: (a) uniform elongation (eu) and (b) total elongation (ef).Fig. 9. Schematic illustrating the procedure for calculating of the strain rate sensitivity, m, for a down jump from 10À1/s to 10À2/s), for DP590 at anengineering strain of 0.1 (true strain of 0.095). For an isotropic material, the von Mises effective stress and strain are equal to rb and et, respectively. Because the DPsteels tested here exhibit normal anisotropy, corrections were made for the known normal anisotropy parameters, r2 (thenormal anisotropy was measured using thinned samples at the uniform strain), shown in Table 3 and best-ﬁt values ofthe material parameter anisotropy parameter a corresponding to the Hill 1979 non-quadratic yield function (Hill, 1979):
- 11. 1756 J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 2ð1 þ r 2 Þra ¼ ð1 þ 2r 2 Þjr1 À r2 ja þ jr1 þ r2 ja ð8Þ The equations for obtaining the appropriate tensile effective stresses and strains for a balanced biaxial stress state havebeen presented (Wagoner, 1980): 2r1 r¼ ; ¼ e1 ½2ð1 þ r 2 Þ1=a e ð9Þ ½2ð1 þ r 2 Þ1=awhere e1 is half of the absolute value of the thickness strain. The value of a was found for each material using Eq. (9) andequating the effective stress and strain from a tensile test and bulge test at an effective strain equal to the true uniform strainin tension for each material, Table 3.3.6. Coupled thermo-mechanical ﬁnite element procedures The proposed constitutive equation was tested using a thermo-mechanical FE model of a tensile test with the same spec-imen geometry as in the experiments. ABAQUS Standard Version 6.7 (ABAQUS, 2007) was utilized for this analysis. One halfof the physical specimen is shown in Fig. 10 with thermal transfer coefﬁcients, but only one-quarter of the specimen wasmodeled, as reduced by mirror symmetry in the Y and Z directions. Eight-noded solid elements (C3D8RT) were used for cou-pled temperature-displacement simulations with two element layers through the thickness. The grip was modeled as a rigidbody. A von Mises yield function and the isotropic hardening law were adopted for simplicity in view of the nearly proportionaluniaxial tensile stress path throughout most of the test and the normal anisotropy values near unity for the DP steels, TableFig. 10. FE model for tensile test: (a) schematic of the model with thermal transfer coefﬁcients, (b) central region of the mesh before deformation and (c)central region of the mesh after deformation.
- 12. J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 17573. The 2% tapered specimen geometry required for experimental reproducibility automatically initiates plastic strain local-ization at the center of the specimen without introducing numerical defects for that purpose. The total elongation (ef) fromeach simulation was deﬁned by the experimental load drop at failure. The simulation accuracy was evaluated based on thecomparison of total elongation with experiments at this same load.3.7. Determination of thermal constants For thermal–mechanical FE simulation, various thermal constants are required. The following constants were determinedusing JMatPro (Sente-Software, 2007) based on chemical composition: thermal expansion coefﬁcient: linear variation from1.54 Â 10À6/K at 25 °C to 1.58 Â 10À6/K at 200 °C, heat capacity: linear variation from 0.45 J/gK at 25 °C to 0.52 J/gK at 200 °C,and thermal conductivity: piecewise linear variation of 36.7 W/m K at 25 °C, 36.9 W/m K at 70 °C, 36.8 W/m K at 100 °C and36 W/m K at 200 °C. Heat transfer coefﬁcient of metal–air contact was measured as 20W/m2 K and heat transfer coefﬁcientof metal–metal contact were taken from the literature as 5 KW/m2 K (Burte et al., 1990). A fraction of the plastic work done during deformation is converted to heat, with the remainder stored elastically as de-fects (Hosford and Caddell, 1983). The relationship between adiabatic temperature rise and plastic work is as follows: Z g DT ¼ rdep ð10Þ qC pwhere g is a fraction of heat conversion from plastic deformation, q is density of the material and Cp is heat capacity at con-stant pressure. In order to measure g for DP steels, temperatures were recorded during tensile tests using three thermocou-ples that were capacitance discharge welded onto specimens on the longitudinal centerline at locations at the center and±5 mm from the center. The specimen was wrapped with glass ﬁber sheet to establish quasi-adiabatic conditions at a strainrate of 5 Â 10À2/s. Fig. 11 shows the results for DP590 and the acceptable correspondence to a value of 0.9 for the parameterg. g was measured only for DP590, but the value 0.9 was used for each of the three materials.4. Results and discussion4.1. Determination of best-ﬁt constitutive constants As shown by the experimental points shown in Fig. 12, the strain rate sensitivity index, m, is not independent of strainrate for any of the steels, so the power-law model (Eq. (B.8)) and Johnson–Cook rate law (Eq. (B.9)) were rejected as inad-equate. The Wagoner rate law (Eq. (B.10)) and a simpliﬁed version the Wagoner law with a linear variation of m with log-arithmic value of strain rate, Eq. (11) below, represent the data equally over this strain rate range as shown in Fig. 12, so thesimpler law was selected: c2 þðc1 =2Þ logðeÁe0 Þ _ _ e_ r ¼ re_ 0 _ ð11Þ e0where re0 is a stress at e0 and c1 and c2 are material constants. _ _ The linear variation law, Eq. (11), had slightly better correlation coefﬁcients (R2 = 0.94–0.99) than those for the Wagonerrate law (R2 = 0.82–0.97). The best-ﬁt values for the parameters for each model are shown in Table 4. 800 30 DP590 True Stress -2 dε/dt: 5X10 /s Temp. Increase (deg. C) True Stress (MPa) 600 20 Temp. increase 400 Eq.10, η=1 Eq.10, η=0.9 10 200 Experiment 0 0 0 0.02 0.04 0.06 0.08 0.1 0.12 True Strain Fig. 11. Flow stress and temperature increase during a tensile test at a nominal strain rate of 5 Â 10À2/s, DP590.
- 13. 1758 J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 Strain rate sensitivity index, m-value 0.02 DP590(Expt.) DP780(Expt.) 0.015 DP980(Expt.) DP590(Fit by Eq. B.10) DP780(Fit by Eq. B.10) DP980(Fit by Eq. B.10) 0.01 0.005 0 -5 -4 -3 -2 -1 10 10 10 10 10 1 Strain rate, d ε /dt (1/sec ) (a) Strain rate sensitivity index, m-value 0.02 DP590(Expt.) DP780(Expt.) DP980(Expt.) 0.015 DP590(Fit by Eq. 11) DP780(Fit by Eq. 11) DP980(Fit by Eq. 11) 0.01 0.005 0 -5 -4 -3 -2 -1 10 10 10 10 10 1 Strain rate, dε /dt (1/sec ) (b)Fig. 12. Measured strain rate sensitivities, m, and their representation by strain rate sensitivity laws: (a) Wagoner rate law (Wagoner, 1981a) and (b)linearized version of Wagoner rate law.Table 4Parameters describing the strain rate sensitivity according to three laws. Power law (mavg) Wagoner rate law Linear law m1 m0 c1 c2 DP590 0.0062 0.162 0.0125 0.0020 0.0103 DP780 0.0050 0.378 0.0263 0.0030 0.0115 DP980 0.0041 0.289 0.0148 0.0021 0.0086 The remainder of the H/V law was ﬁt using results from continuous, isothermal tensile tests in the uniform strain rangeconducted at a strain of 10À3/s and at three temperatures: 25, 50, and 100 °C, Fig. 13 (Note that the H/V model reproduces thevariation of strain hardening rate in the application range 25 °C–100 °C, one of the key objectives of this work.). In order tochoose a suitable form for the thermal softening function h(T), three forms were initially compared as shown in Fig. 14:Linear (Eq. (B.11)), Power Law 1 (Eq. (B.12)), and Johnson–Cook (Eq. (B.14)). As shown in Fig. 14, and not unexpectedly, thereis no signiﬁcant difference in the accuracy of the ﬁts of these three laws over the small temperature range tested. The Linearmodel (Eq. (B.11)) was chosen for the current work as perhaps the more common and simpler choice, but no advantage isimplied. For application over a larger temperature range or for other materials, presumably one of the forms shown inAppendix B would provide a measurable advantage over the others and thus could be adopted. With the form of the thermal function determined, the eight optimal coefﬁcients (a1, a2, HHV, nHV, VHV, AHV, BHV, b) may bedetermined for the combined function, again using results from the three tensile tests (at three temperatures) for eachmaterial:
- 14. J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 1759 1200 DP980 True Stress (MPa) 1000 H/V Model DP780 800 50 deg. C 25 deg. C 100 deg. C DP590 600 Experiment -3 dε/dt: 10 /s 400 0.02 0.04 0.06 0.08 0.1 0.12 0.14 0.16 True Strain Fig. 13. Comparison of isothermal tensile test data and best-ﬁt H/V model for DP590, DP780, and DP980. 1080 Line h(T) S.D. (MPa) Eq. B.11 0.4 Eq. B.12 1.2 1060 True Stress (Mpa) Eq. B.14 0.4 1040 Experiment 1020 DP980 -3 dε/dt: 10 /s, ε: 0.09 1000 0 20 40 60 80 100 120 Temp (deg. C) Fig. 14. Comparison of temperature dependent functions h(T) for DP980. f ðe; TÞ Á hðTÞ ¼ ½aðTÞðHHV enHV Þ þ ð1 À aðTÞÞV HV ð1 À AHV eÀBHV e Þ Á ½1 À bðT À T 0 Þ ð12Þ 8 Using the method of least squares, high and low values of each variable were selected as initial values, producing 2 setsof starting sets of parameters. The approximate range of parameters were known with Hollomon and Voce ﬁt with the mate-rial data, therefore the initial values of each parameter were selected based on the range. If ﬁt values are out of the range,new initial values were selected and ﬁt again. The initial values are shown in the Table 5. Best-ﬁt coefﬁcients were found foreach starting set when the absolute value of the difference between the norm of the residuals (square root of the sum ofsquares of the residuals), from one iteration to the next, was less than 0.001. The set exhibiting the minimum R2 valuewas chosen as optimal, as reported in Table 5. The accuracy of the ﬁt is shown in Table 5 as a standard deviation betweenexperiment and ﬁt line and illustrated graphically in Fig. 13. Using identical procedures, except for the RK model which was ﬁt according to a procedure recommended by provided byits originators (Rusinek, 2009), several alternative constitutive models were ﬁt to the same tensile test and jump test data, asfollows:1. H/V model with a = 1 (Hollomon strain hardening at all temperatures).2. H/V model with a = 0 (Voce strain hardening at all temperatures).3. H/V model with best-ﬁt constant a = ao (H/V strain hardening, independent of temperature).4. Lin–Wagoner (LW) model (Eq. (A.7)) (Voce hardening dependent on temperature).5. Rusinek–Klepaczko (RK) model (Eq. (A.10), (A.11)) (Power-law hardening dependent on temperature). These choices were made to be representative of the major classes of constitutive models, as reviewed in Section 1.2.Models 1 and 2 are power-law and saturation hardening models, respectively, that are independent of temperature (exceptfor a multiplicative function to adjust ﬂow stress with temperature). Models 3 and 4 allow strain hardening rates to varywith temperature within the frameworks of saturation/Voce or power-law/Hollomon forms, respectively.
- 15. 1760 J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771Table 5Trial and best-ﬁt coefﬁcients of the H/V model. Trial values fH fV Temp. const. R2 Parameters Low High S.D.(MPa) DP590 HHV 500 1500 HHV: 1051 VHV: 643.9 a1: 0.818 0.999 nHV 0.05 0.25 nHV: 0.179 AHV: 0.576 a2: 0.00193 S.D. = 0.5 VHV 500 1500 BHV: 22.44 b: 2.7 Â 10À4 AHV 0.1 0.6 BHV 10 40 a1 0.1 0.9 a2 0 0.005 b 0 0.005 DP780 HHV 500 2000 HHV: 1655 VHV: 752.1 a1: 0.507 0.998 nHV 0.05 0.25 nHV: 0.213 AHV: 0.265 a2: 0.00187 S.D. = 2.5 VHV 500 1500 BHV: 30.31 b: 5.8 Â 10À4 AHV 0.1 0.6 BHV 10 40 a1 0.1 0.9 a2 0 0.005 b 0 0.005 DP980 HHV 500 2000 HHV: 1722 VHV: 908.1 a1: 0.586 0.999 nHV 0.05 0.25 nHV: 0.154 AHV: 0.376 a2: 0.00149 S.D. = 0.6 À4 VHV 500 1500 BHV: 39.64 b: 3.9 Â 10 AHV 0.1 0.6 BHV 10 40 a1 0.1 0.9 a2 0 0.005 b 0 0.005 The material parameters for the RK model, Eq. (A.10), were found using a procedure consisting of six steps recommendedby the ﬁrst author (Rusinek, 2009). Some fundamental constants in RK model: maximum strain rate, minimum strain rateand melting temperature were ﬁrst to be taken from the literature (Larour et al., 2007) and the elastic modulus was takento be constant because this study only covered the small homologous temperature range. The remaining six steps followedfor ﬁtting the RK model are as follows: Step 1: rÃ ðeP ; TÞ in Eq. (A.11) is zero at low strain rate and at critical temperature. In this study rÃ ðeP ; TÞ ¼ 0 at the strain _ _ rate of 10À4/s and the temperature of 300 K since those were the lowest values for strain rate and temperature in this work. Using this strain rate and temperature combination, C1 was calculated. Step 2: Eq. (A.10) was ﬁt to material data at the strain rate of 10À4/s and temperature of 300 K, in which rÃ ðeP ; TÞ ¼ 0, thus _ allowing determination ofA ð10À4 ; 300 KÞ and n ð10À4 ; 300 KÞ. Step 3: The strain rate sensitivity term, rÃ ðeP ; TÞ, was ﬁt to jump test results in order to determine C0 and m. _ Step 4: Aij ðei ; T j Þ and nij ðei ; T j Þ were found at each strain rate and temperature using Eq. (A.10),. _ _ Step 5: Aðe; TÞ was ﬁt to Aij values to ﬁnd A0 and A1. _ Step 6: nðe; TÞ was ﬁt to nij values to ﬁnd B0 and B1. _ The optimal ﬁt coefﬁcients, standard deviations, and R2 values of all models are shown in Tables 6 and 7. The true stress–strain curves for each of these ﬁts for DP780 are shown in Fig. 15. While the differences are small in theuniform tensile range (consistent with the small standard errors of ﬁt shown in Tables 5–7), the differences become apparentwhen extrapolated to higher strains. Strain hardening at strains beyond the tensile uniform range is particularly importantfor sheet forming applications with high curvature bending, where bending strains can be large. The transition of strain hard-ening type of the H/V law from more Hollomon-like at room temperature to progressively more Voce-like behavior at 50 and100 ° C can be seen by comparing Figures 13a, 13b and 13c. Tables 5–7 show that the H/V model provided the lowest standard deviations of ﬁt for each material, followed progres-sively by the three H/V models with constant a, the LW model, and then the RK model. The difﬁculty of ﬁtting RK model tothe DP steel data has a fundamental origin: the data showed the strain hardening increases with increasing strain rate butdecreases with increasing temperature, while the RK model requires that the effects of increasing strain rate and tempera-ture have the same sign of effect on the strain hardening rate.4.2. Comparison of constitutive model predictions with hydraulic bulge tests Fig. 16 compares the various constitutive models established above from tensile data with results from room-tempera-ture (25 °C) hydraulic bulge tests. It is apparent visually and from the standard deviations computed over the strain range
- 16. J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771 1761Table 6Best-ﬁt coefﬁcients of H/V model for a(T) = 1, a(T) = 0, and a(T) = a0. a(T) = 1a a(T) = a0 b a(T) = 0 a f(e)h(T) R2 f(e)h(T) R2 f(e)h(T) R2 S.D.(MPa) S.D.(MPa) S.D.(MPa) DP590 H1: 1039 0.998 a0: 0.875 0.999 V0: 761.45 0.999 n1: 0.186 S.D. = 2.5 H1: 983 S.D. = 0.9 A0: 0.452 S.D. = 2.0 b: 5.4 Â 10À4 n1: 0.166 B0: 14.6 V0: 806.9 b: 5.6 Â 10À4 A0: 0.825 B0: 22.4 b: 5.5 Â 10À4 DP780 H1: 1234 0.997 a0: 0.850 0.997 V0: 940.9 0.997 n1: 0.148 S.D. = 3.2 H1: 1147 S.D. = 2.8 A0: 0.370 S.D. = 3.2 b: 1.0 Â 10À3 n1: 0.175 B0: 17.19 V0: 1521 b: 1.0 Â 10À3 A0: 0.289 B0: 37.7 b: 1.0 Â 10À3 DP980 H1: 1486 0.996 a0: 0.707 0.999 V0: 1111 0.997 n1: 0.135 S.D. = 3.9 H1: 1332 S.D. = 1.3 A0: 0.353 S.D. = 3.2 b: 7.4 Â 10À4 n1: 0.125 B0: 24.33 V0: 2154 b: 7.4 Â 10À4 A0: 0.9 B0: 52.3 b: 7.4 Â 10À4 a For a(T) = 1 and a(T) = 0, the same initial values in Table 5 were used. b For a(T) = a0, the same initial values in Table 5 were used except V0, A0 and B0 which were found out of the range. For these three parameters, 500 and2500 MPa, 0.1 and 0.9, and 10 and 60 were used for initial values, respectively.Table 7Trial and best-ﬁt coefﬁcients of LW and RK models. LW RK Trial Values f(e)h(T) R2 f(e)h(T) S.D.(MPa) S.D. (MPa) DP590 A: 500, 1500 A: 764.5 0.999 A0: 1072 Tm: 1750 K S.D. = 4.2 B: 0.1, 0.6 B: 0.452 S.D. = 2.5 A1: 0.076 emax : 107 =s _ C1: À5, À40 C1: À14.3 e0: 0 emin : 10À5 =s _ C2: À0.2.0 C2: À0.010 B0: 0.184 b: À0.9, À0.1 b: À0.229 B1: À0.043 C0:180.6 C1:0.53 m: 1.53 A0: 1381 A1: 0.245 DP780 A: 500, 1500 A: 960.4 0.998 e0: 0 Tm: 1750 K S.D. = 9.9 B: 0.1, 0.6 B: 0.375 S.D. = 2.7 B0: 0.146 emax : 107 =s _ C1: À5, À40 C1: À15.2 B1: À0.033 emin : 10À5 =s _ C2: À0.2. 0 C2: À0.102 C0: 404.3 b: À0.9, À0.1 b: À0.609 C1: 0.53 m: 2.11 DP980 A: 500, 1500 A: 1118 0.999 A0: 1575 Tm: 1750 K S.D. = 10 B: 0.1, 0.6 B: 0.353 S.D. = 1.8 A1: 0.140 emax : 107 =s _ C1: À5, À40 C1: À23.3 e0: 0 emin : 10À5 =s _ C2: À0.2. 0 C2: À0.032 B0: 0.134 b: À0.9, À0.1 b: À0.311 B1: À0.025 C0: 289.6 C1: 0.53 m: 1.920.03–0.7, 0.03–0.34, and 0.03–0.23 for DP590, DP780 and DP980, respectively, that the full H/V model and H/V model withthe best-ﬁt constant a0 value (independent of temperature) extrapolated to higher strains reproduce the hydraulic bulge testresults with much greater ﬁdelity than either Hollomon or Voce hardening models. Note that the experimental stress–strain
- 17. 1762 J.H. Sung et al. / International Journal of Plasticity 26 (2010) 1746–1771behavior for these materials is intermediate between standard Voce and Hollomon laws, and further that the H/V law ﬁtfrom the tensile predicts the high-strain behavior much better than the standard ones. This result illustrates the achievementof one of the principal objectives of the current development predicting large strain, stress–strain curves accurately. It wouldbe desirable to have data like that shown in Fig. 16 at other temperatures. Unfortunately, the authors are unaware of anyfacility capable of elevated temperature balanced biaxial testing of high strength steels. 1100 DP780 Temp: 25 deg. C Effective Stress (MPa) -3 1000 dε/dt: 10 /s 900 α(T)=1 α(T)=αo α(T)=0 800 Tensile Test LW RK H/V 700 0.1 0.2 0.3 Effective Strain (a) 1100 DP780 Temp: 50 deg. C True Stress (MPa) -3 1000 dε/dt: 10 /s Tensile Test 900 α(T)=1 α(T)=αo α(T)=0 800 LW RK H/V 700 0.1 0.2 0.3 True Strain (b) 1100 α(T)=1 DP780 α(T)=αo Temp: 100 deg. C α(T)=0 True Stress (MPa) -3 1000 dε/dt: 10 /s LW RK H/V 900 800 Tensile Test 700 0.1 0.2 0.3 True Strain (c) Fig. 15. Comparison of selected constitutive models at various temperatures, DP780: (a) 25 °C, (b) 50 °C and (c) 100 °C.

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment